234 Elasticity and transverse Strength [Augt, 
Number of tbe 
experiments. 
Names of the 
woods. 
Specific gravity.! 
elasticity per- 
fect. 
Breaking weight 
in lbs. 
Ultimate deflec- 
tion in inches. 
Value of 
U, or 
A 
Value of 
E, or 
/® W / 
Value of 
S, or 
AV 
Weight 
in lbs. 
Deflec- 
tion in 
inches. 
d& 
4 ad 2 
412 
Lance wood or 
863 
200 
.6 
520 
1.25 
413 
Maina-baun. 
900 
250 
.55 
978 
3.85 
414 
Specimen 
873 
250 
.575 
884 
4.0 
415 
66 inches long. 
869 
250 
.55 
1039 
4.2 
60 ,, bearing. 
2X14 inches. 
C=lbs. 28,737. 
Mean results 
876 
250 
.568 
855 
3.325 
540 
7922500 
2137 
416 
Koossum. 
1098 
400 
1.1 
756 
2.35 
417 
Fresh from Jynu- 
1102 
400 
1.1 
652 
6.8 
418 
ghur Timber Agen- 
1073 
450 
1.1 
1123 
4.5 
419 
cy, September 1828 
1064 
450 
1.275 
768 
2.75 
C=lbs. 18,121. 
Mean results 
1084 
240 
1.14 
825 
4.1 
632 
9208000 
1856 
420 
Kussoomah. 
1108 
250 
.95 
861 
4.2 
421 
Fresh from Jynu- 
1075 
250 
.975 
809 
3.8 
422 
ghur Timber Agen- 
1084 
250 
1.075 
809 
4.6 
423 
cy, September 1828 
1098 
250 
1.1 
756 
4.1 
C=lbs. 14,790. 
Mean Tesults 
1091 
250 
1.0 
809 
4.2 
617 
5832000 
1820 
42b 
Paundur. 
764 
250 
.95 
835 
4.0 
426 
Fresh from Jynu- 
838 
250 
.85 
756 
2.9 
427 
ghur TimberAgen- 
739 
250 
.85 
809 
4.5 
428 
cy, September 1821: 
742 
250 
.95 
704 
4.8 
C'=lbs. 15,564. 
Mean results 
771 
250 
.9 
776 
4.0 
648 
6480000 
1746 
383 
Dhoree. 
716 
200 
.725 
704 
6.0 
384 
Fresh from J ynu - 
706 
200 
.625 
650 
3.6 
385 
ghurTimber Agen- 
735 
200 
.425 
661 
3.2 
386 
cy, September 1821 
904 
200 
.95 
585 
4.2 
387 
C=lbs. 13,694. 
700 
200 
.875 
672 
4.6 
388 
700 
200 
.775 
69 5 
4.2 
Mean results 
744 
200 
.73 
661 
4.3 
602 
6391000 
1487 
429 
Assaun. 
946 
300 
.875 
844 
5.4 
430 
Fresh from Jynu- 
930 
300 
.875 
844 
5.4 
431 
ghurTimber Agen- 
1000 
300- 
.875 
913 
70 
432 
cy, September 1828 
1069 
300 
.875 
1012 
6.1 
C=lbs, 17,690. 
Mean results 
986 
300 
.875 
903 
6.0 
432 
7997000 
2032 
